Nanowires for Dissipation-less Spintronics
Amrita Singh, Charlotte Jansen, Kaveh Lahabi, and Jan Aarts* Huygens-Kamerlingh Onnes Laboratory, Leiden University,
P.O. Box 9504, 2300 RA Leiden, The Netherlands (Received 29 June 2016; published 18 October 2016)
Superconductor-ferromagnet (S-F) hybrids based on half-metallic ferromagnets, such as CrO2, are ideal candidates for superconducting spintronic applications. This is primarily due to the fully spin-polarized nature of CrO2, which produces enhanced long-range triplet proximity effects. However, reliable production of CrO2-based Josephson junctions (JJs) has proved to be extremely challenging because of a poorly controlled interface transparency and an incomplete knowledge of the local magnetization of the CrO2films. To address these issues, we use a bottom-up approach to grow CrO2nanowires on prepatterned substrates via chemical-vapor deposition. A comprehensive study of the growth mechanism enables us to reliably synthesize faceted, homogeneous CrO2wires with a well-defined magnetization state. Combining these high-quality wires with a superconductor produces JJs with a high interface transparency, leading to exceptionally large 100% spin-polarized supercurrents, with critical current densities exceeding109Am−2 over distances as long as 600 nm. These CrO2-nanowire-based JJs thus provide a realistic route to creating a scalable device platform for dissipation-less spintronics.
DOI:10.1103/PhysRevX.6.041012 Subject Areas: Spintronics, Superconductivity
Ferromagnetic nanostructures have emerged as a leading candidate for spintronic applications because of their ability to carry spin-polarized currents[1,2]. However, one of the biggest challenges facing the field of spintronics is the large amount of dissipation that is generated by current-driven processes at the nanoscale[3,4]. One way to address this issue is to combine a ferromagnet (F) with a supercon-ductor (S) to produce supercurrents in the ferromagnet. This method seems counterintuitive since electron spins in the Cooper pair are aligned antiparallel in a superconductor, while a ferromagnet prefers parallel spins. However, it has been shown that by engineering the S-F interface, supercurrents can indeed be injected into the ferromagnet
[5–11]. The novelty of this induced supercurrent lies in its spin-polarized nature [12–14]. Such spin-polarized triplet Cooper pairs can only be generated when singlet Cooper pairs at the S-F interface are subjected to spin mixing and rotation, usually achieved by introducing an additional thin ferromagnetic layer at the interface [9,10,16,17]. Since triplet Cooper pairs are not affected by the exchange field of the ferromagnet, they can survive over considerably long distances, thereby giving rise to spin-polarized supercurrents.
Half-metallic ferromagnets are fully spin polarized and are expected to enhance the generation of triplet Cooper pairs , making them an ideal material choice for dissipation-less spintronics. This idea is indeed supported by experimental studies of CrO2, a well-known half-metallic ferromagnet. S-F-S Josephson junctions fabricated on films of CrO2 have been shown to carry large super-currents . Furthermore, the spatial extent of induced triplet correlations in CrO2 is of the order of a micron
[19,20], while it is limited to a few tens of nanometers
for standard ferromagnets (Ni, Co, Fe). Finally, recent experiments in a spin-valve geometry [21,22] provide direct evidence that triplet generation is enhanced by more than an order of magnitude in CrO2, as compared to other ferromagnets.
Despite the fact that CrO2clearly holds great promise for superconducting spintronics, progress in this field has been impeded because of a poorly controlled S-F interface transparency, ill-defined current paths, and an incomplete knowledge of the local magnetization state associated with full films of CrO2. Here, we show that all of these problems can be circumvented by growing high-quality CrO2 nano-wires via selective area growth. We show that a thorough understanding of the growth process is vital for the generation of high-quality S-F-S JJs. By studying the effects of confinement, growth time, and crystal orientation on the magnetic and structural morphology of these structures, we demonstrate the reliable growth of homo-geneous, crystalline nanowires with a desired geometry and magnetization state. This robust control over the magneti-zation and transparency enables us to reproducibly fab-ricate CrO2-based JJs with record-high critical current *firstname.lastname@example.org
densities, and thus, it represents a crucial step towards the realization of a scalable superconducting spintronics device platform based on half-metallic ferromagnets.
It has been shown that full films of CrO2can be grown epitaxially via chemical-vapor deposition (CVD) [23,24]. One might imagine that the most convenient way to create CrO2structures with a well-defined geometry would be to follow a top-down approach by etching away selected portions of the full film. However, etching damages the edges of the structure. Furthermore, full-film growth results in the creation of a large number of grain boundaries, which remain present in the final device [see Fig. 1(f)] and are likely to reduce into insulating Cr2O3, thus suppressing current and supercurrent flow. It is therefore desirable to create these structures via a bottom-up approach such as selective area growth (SAG). SAG relies on the fact that CrO2is only known to grow epitaxially on TiO2or sapphire substrates. Thus, a patterned SiOx mask can be used to define the geometry of the CrO2nanostructures as shown in Fig.1(a)(details of the growth are provided in the Methods section). The growth of CrO2nanowires proceeds through two important stages, as discussed below.
The initial stage of growth involves the nucleation and growth of CrO2 inside the trench [see schematic in Fig.1(a)]. A detailed understanding of this stage is essential to identify the parameters that affect the quality of the crystal. In order to probe this stage, the wires were grown for 20 min, which is just enough to fill the 25-nm-deep SiOx trench. Figures1(b)–1(f)show the scanning electron microscopy (SEM) images of nanowires with trench width
wtrvarying from 230 nm to2μm. The L shape is chosen in order to compare the growth along different crystallo-graphic axes. Along the (001) axis, we find that the growth is homogeneous for smaller trench widths (230 nm and
530 nm), but it becomes increasingly inhomogeneous for the wider trenches (1μm and 2μm). The explanation for this lies in the fact that the nucleation of CrO2 occurs preferentially at the SiOx=TiO2 interface, followed by propagation of the growth front towards the center of the trench. This process is self-limited and is characterized by a length scale λ bearing resemblance to a surface diffusion length. Therefore, if wtr<2λ, the growth is homogeneous [Figs.2(b)and 2(c)], whereas for wtr>2λ a void is formed at the center of the trench [Figs. 2(d)
and2(e)]. Growth along the (010) axis follows a similar mechanism for wtr>2λ, but for narrower trenches, we observe a different type of inhomogeneous filling, in which vertical growth along the wall is followed by inward lateral growth (see Ref.). We note that our studies are quite different from earlier reports, where it was assumed that CrO2nucleates and grows uniformly in the narrow trenches away from the SiOx side walls.
As the growth time is increased, the CrO2begins to grow laterally above the SiOxmask [see Fig.2(a)], accompanied by a significant change in its surface morphology. The most striking observation is the appearance of well-defined crystal facets, which (as will be shown later) provide an excellent interface for CrO2-based JJs. Figures 2(b)–2(d)
show the evolution of such facets with the growth time (tg), upon deposition in disk-shaped trenches. Fortg¼20 min,
growth is restricted to the (circular) trench, resulting in the formation of CrO2 disks. With a further increase in tg (25 min), CrO2 starts to overgrow laterally on SiOx, and
 facets begin to appear, presumably to minimize the total surface energy. For tg¼45 min, the CrO2 islands exhibit fully developed facets with smooth surfaces. This type of facet evolution with growth time has been reported recently for SAG of GaN.
FIG. 1. Early stage growth of CrO2wires. (a) Schematic of edge-enhanced nucleation and growth of CrO2inside a SiOxtrench. SEM
In addition to the formation of crystalline facets, the extent of lateral overgrowth naturally determines the effective dimensions of the CrO2 structures. We quantify this by studying the CrO2growth in SiOxtrenches oriented
along different crystallographic directions. Figure 2(e)
shows a SEM image of CrO2 wires grown in 500-nm-wide trenches for 45 min. It is clear that the extent of overgrowth depends strongly on orientation of the wire; however, it hardly depends on the trench width (see Fig.2
of Ref. ). The anisotropy of lateral overgrowth with SAG has been reported earlier for thick CrO2 structures
[26,28]. However, from our data, we can extract
quantita-tive information about the anisotropy, which is important for the accurate determination of critical current density in S-F-S JJs.
In Fig.2(f), we plot the average wire width as a function ofθ[angle relative to the (010) axis] for differenttg. The anisotropy is largest for tg ¼45 min and reduces with a
decrease in tg. The maximum lateral overgrowth occurs roughly atθ¼60°, the direction which coincides with the diagonal of the CrO2 unit cell. The height of the wires reaches a minimum at this angle, not unexpectedly, since lateral overgrowth occurs at the expense of vertical growth. This result is in contrast with the previous reports on SAG of CrO2structures where vertical overgrowth was reported to be isotropic. This correlation between vertical and lateral growth can be understood on the basis of a mass transport mechanism and is explained in more detail in Ref. .
Our discussion thus far clearly shows that we can grow high-quality, homogeneous, and crystalline wires of CrO2. The controlled growth of these wires along specific crystallographic directions allows us to exploit the shape anisotropy to reliably create specific magnetization states, a
vital ingredient for the generation of triplet supercurrents. It is known that for CrO2films, the magnetic hard (easy) axis is aligned along the 010 (001) axis[26,29,30]. Figure3(a)
shows a magnetic force microscopy (MFM) image of CrO2 wires grown along different crystallographic orientations. Away from the easy axis, striplike domains form in order to minimize the total magnetic energy. This is seen as alternating bright or dark contrast in the MFM image, and more clearly as oscillations in the magnetic phase contrast [Fig. 3(b) top and middle panels]. However, the wire oriented along (001) is in a single domain state, evident from the absence of contrast in the MFM image and the representative line scan along this direction
5 µm (001)
(a) (b) (c)
(e) (f ) (g)
1.2 µm 250 nm 260 nm
tg= 20 mins tg= 25 mins tg= 45 mins
0 30 60 90
0.5 1.0 1.5 2.0
tg= 45 mins
tg= 35 mins
tg= 25 mins
θ(degree) tg= 20 mins
FIG. 2. Lateral overgrowth and facet evolution. (a) Schematic of lateral epitaxial overgrowth of CrO2over SiOxfor higher growth
times. Scanning electron micrographs of CrO2structures, all grown in circular SiO2trenches, for (b) 20 min (filling the disk-shaped trench), (c) 25 min, and (d) 45 min. The latter two are overgrowth structures. (e) Scanning electron micrographs of CrO2nanowires oriented between θ¼0° (010) andθ¼90° (001) at the intervals of 15° and grown in 500-nm-wide trenches for 45 min. Angular dependence of (f) width and (g) height of CrO2 nanowires, grown in 500-nm-wide SiOx trenches, for different growth times.
0 4 8
0 4 8
0 2 4 6
0 4 8
Line scan 3 Line scan 2
Line scan 1
Line scan 1
FIG. 3. Tuning magnetic domains by shape anisotropy. (a) Mag-netic force micrograph of CrO2nanowires grown in 500-nm-wide trenches, oriented betweenθ¼0° andθ¼90° at intervals of 15°. White lines along the edges of the wires represent the line scan used to determine the magnetic phase contrast. Prior to MFM measurements, the samples were first magnetized with a 1-T field along the easy axis, followed by setting the field to−8mT along the same axis. (b) Magnetic phase contrast along the edges of the wires for θ¼0° (upper panel), θ¼45° (middle panel), and
[Fig.3(b)bottom panel]. We use these high-quality CrO2 wires grown along the easy axis to create S-F-S JJs. It is important to stress here that such local control over the magnetization is impossible to achieve in full films (see Fig. 3 of Ref.), reflecting directly in a larger spread in performance of JJ devices.
While the crystalline facets of our CrO2wires grown via SAG provide transparent S-F interfaces, the uniform magnetization of the wire enables us to reliably engineer the magnetic inhomogeneity at the interface. This is achieved through the deposition of a Ni wire (mixer layer). The shape anisotropy of the Ni layer is such that its magnetization is perpendicular to the CrO2 wire [see schematic in Fig.4(a)]. This ensures the maximum possible magnetic noncollinearity at the S-F interface, resulting in efficient triplet Cooper pair generation. The mixer layer is part of a trilayer contact consisting of Cu (or Ag), Ni, and the superconductor (amorphous MoGe) (see Methods section for fabrication details). The Cu (or Ag) prevents exchange coupling between CrO2 and Ni, while MoGe induces the proximity effect. Figure 4(a) shows a SEM image (false color) of a JJ device. We present results from two JJs (J1 and J2) whose device parameters are summa-rized in Table 1.
Figure4(b)shows a plot of resistance (R) vs temperature (T) for J1 measured in quasi-4 probe geometry. Around
T¼6.5K,R drops sharply because of the superconduct-ing transition in the MoGe leads. Coolsuperconduct-ing further (below
5 K), the JJ reaches a zero resistance state [inset Fig.4(b)] accompanied by the appearance of a supercurrent. The measured resistance of the device is dominated by the Cu layer in the leads since the Cu specific resistivityρ0;Cu of the order of 5μΩcm is much smaller than ρ0;MoGe≈ 200μΩcm. Taking a length of 70μm per lead, a width of2.5μm, and a thickness of 5 nm, we find 560Ω. The normal resistance of the CrO2weak link we estimate using ρ0;CrO2≈6μΩcm (along the easy axis) to be0.32Ω. This
leaves about 20Ω as the contact resistance. We note in Fig.4(b)that the low-temperature R is well below0.32Ω. Figure4(c)showsI-Vcharacteristics of J1 at a few different temperatures and is used to extract the critical current. The voltage increase just above Ic starts with a small steep
slope, but then it settles to a slope that is close to0.3Ω, quite as expected for the CrO2weak link. The value of Ic, along with a precise knowledge of the dimensions of CrO2 wires, allows us, for the first time, to reliably estimate the critical current density (Jc) of CrO2-based JJs. In Fig.4(d), we plot the variation ofJc with temperature for J1 and J2. Below 5 K, Jc reaches values in excess of 109 Am−2. Interestingly, despite its larger junction length (see Table1), J2 has a significantly larger critical current density than J1. We believe that this enhancement results from a higher interface transparency due to the use of Ag, which, unlike Cu, does not form oxides at the interface with CrO2. The critical current density for our JJs is an order of magnitude higher than standard S-F-S JJs[17,31], despite the fact that our devices are almost 100 times longer, supporting the notion that exceptionally large triplet supercurrents can be generated in half-metallic ferromagnets. The device lengths are also significantly larger than the typical mean free path of CrO2, which is of the order of 50 nm [15,32]; therefore, our JJs are in the diffusive long junction limit. It has been theoretically predicted that the temperature dependence of the critical current of CrO2-based JJs would exhibit a peak at low temperature, and the position of the peak is determined by the junction length. Since our junction lengths are very long, we expect such a peak to occur at temperatures lower than 2 K, which cannot be achieved in our present measurement setup. At the mea-sured temperatures, we expect Jc to be proportional to
thÞ1=2, where Eth is the Thouless energy of the junction. The inset of Fig. 4(d)clearly shows that this is indeed the case for J1, where lnðJcÞ− 3=2lnðTÞvaries linearly with T1=2. The slope of this plot allows us to directly estimateEth∼11μV. Using previous
MCrO2 Cu/AgNi MoGe
FIG. 4. Josephson junctions with CrO2wires. (a) Schematic of Josephson junctions fabricated with CrO2wire as a weak link. We show the scanning electron micrograph (false color) of a Josephson junction on a CrO2nanowire (green). The graph also shows crystal and magnetization directions. Orange contact pads consist of trilayer (Cu or Ag)/Ni/MoGe. (b) ResistanceRversus temperature T for junction J1. The inset shows the behavior around zero resistance. (c) CurrentIversus voltageV character-istics of J1 at different temperatures. (d) Critical current density Jc versus T. The inset shows a linear fit to a plot of
TABLE I. Wire width, wire thickness, and junction length of two Josephson junction devices based on CrO2nanowires.
Device Width Thickness Junction length
J1 (Cu) 1μm 75 nm 400 nm
estimates of the diffusion constantD¼3.7×10−3 m2s−1 from a Fermi velocity of 2.2×105m s−1, and a typical mean free path of 50 nm, we calculateEth¼ℏD=L2to be15μV for our junction length of L¼400nm, in good agreement with our experiments.
In conclusion, we have shown that a detailed under-standing of selective area growth of CrO2 allows us to reliably produce high-quality nanowires with a well-defined geometry and magnetization. Proximizing these wires with a superconductor produces S-F-S Josephson junctions that support record-high triplet supercurrents over long distances. The estimated current densities are large enough to envision devices where such spin-polarized supercurrents could be used to manipulate the magnetiza-tion of a nanomagnet [1,35]. Furthermore, the use of a patterned growth technique would allow one to engineer domain walls at predefined locations [36,37], thereby realizing a scalable device architecture where fully spin-polarized supercurrents could be used to create spintronic devices without dissipation.
Technical support from M. B. S. Hesselberth, D. Boltje, and A. F. Beker is gratefully acknowledged. We also strongly benefited from discussions with S. Goswami. This work is part of the research program of the Foundation for Fundamental Research on Matter (FOM), which is part of the Netherlands Organisation for Scientific Research (NWO). The work was also supported by the EU COST action MP1201“NanoSC”and by a grant from the Leiden-Delft Consortium “NanoFront”.
APPENDIX: METHODS 1. Selective area growth
We start with a rutile (100) TiO2substrate, which has a tetragonal surface net spanned by theb- andc-crystal axes (b¼0.459nm,c¼0.296nm; note thata¼b), on which CrO2 (b¼0.442nm, c¼0.292nm) can be grown iso-structurally. The lattice mismatch is anisotropic, being
−1.4% along the b axis and −3.8% along the c axis. This leads to anisotropic growth rates, which are important for nanowire growth. Substrates were cleaned with organic solvents (Acetone/IPA) followed by HF treatment, on which a 25-nm SiOx thin film was sputter deposited.
Using e-beam resist and lithography, openings of different sizes and shapes were created in the resist along different crystallographic directions. SiOx was selectively removed from the openings using reactive ion etching with a CF4 and an O2plasma. The etch time of SiOxis critical because underetching results in only partial removal of SiOx, while overetching damages the underlying TiO2substrate, which affects the film quality adversely (see Fig. 4 of Ref.). Next, CrO2 was grown selectively in the SiOx trenches (trench widthwtr) by CVD in a two-zone furnace, where the
substrate temperature was kept at 395°C, while the pre-cursor CrO3was heated to260°C in the presence of a flow of 100 sccm O2carrier gas. By monitoring the growth times (tg), samples with varying thicknesses were prepared. Each
sample consists of CrO2 structures with different sizes, shapes, aspect ratios, and orientations. SEM, atomic force microscopy, and MFM were used to examine the structural and magnetic morphology of the CrO2nanostructures. For the MFM measurements, the samples were magnetized in a 1-T field along the easy axis, followed by a decrease of the field to−8 mT in order to create a domain state.
2. Fabrication of lateral Josephson junctions.
To fabricate JJs, trilayer [Cu or Ag (5 nm)/Ni (1.5 nm)/ MoGe (100 nm)] contact pads, defined by electron beam lithography, were sputter deposited on CrO2 wires, fol-lowed by a lift-off process. CrO2is a metastable phase and inevitably reduces to more stable Cr2O3, which is anti-ferromagnetic and insulating. The surface of CrO2is etched
in situwith an argon plasma prior to the sputtering of the
trilayer contact pads, which are deposited without breaking the vacuum. The optimized etching parameters, in combi-nation with faceted CrO2crystals, produced JJS with high interface transparency.
 S. S. P. Parkin, M. Hayashi, and L. Thomas, Magnetic Domain-Wall Racetrack Memory,Science320, 190 (2008).  V. E. Demidov, S. Urazhdin, and S. Demokritov, Direct Observation and Mapping of Spin Waves Emitted by Spin-Torque Nano-Oscillators,Nat. Mater.9, 984 (2010).  J. C. Slonczewski, Current-Driven Excitation of Magnetic
Multilayers,J. Magn. Magn. Mater.159, L1 (1996).  Y. Huai, F. Albert, P. Nguyen, M. Pakala, and T.
Valet, Observation of Spin-Transfer Switching in Deep Submicron-Sized and Low-Resistance Magnetic Tunnel Junctions,Appl. Phys. Lett.84, 3118 (2004).
 F. S. Bergeret, A. F. Volkov, and K. B. Efetov,Long-Range Proximity Effects in Superconductor-Ferromagnet Struc-tures,Phys. Rev. Lett.86, 4096 (2001).
 M. Eschrig, J. Kopu, J. C. Cuevas, and G. Schön,Theory of Half-Metal/Superconductor Heterostructures, Phys. Rev. Lett.90, 137003 (2003).
 M. Houzet and A. I. Buzdin,Long Range Triplet Josephson Effect through a Ferromagnetic Trilayer,Phys. Rev. B76, 060504(R) (2007).
 M. S. Anwar, M. Veldhorst, A. Brinkman, and J. Aarts, Long Range Supercurrents in FerromagneticCrO2Using a Multilayer Contact Structure,Appl. Phys. Lett.100, 052602 (2012).
 J. Wang, M. Singh, M. Tian, N. Kumar, B. Liu, C. Shi, J. K. Jain, N. Samarth, T. E. Mallouk, and M. H. W. Chan, Interplay Between Superconductivity and Ferromagnetism in Crystalline Nanowires,Nat. Phys.6, 389 (2010).  M. Eschrig,Spin-Polarized Supercurrents for Spintronics:
A Review of Current Progress,Rep. Prog. Phys.78, 104501 (2015).
 J. Linder and J. W. A. Robinson, Superconducting Spin-tronics,Nat. Phys. 11, 307 (2015).
 N. G. Pugach and A. I. Buzdin,Magnetic Moment Manipu-lation by Triplet Josephson Current,Appl. Phys. Lett.101, 242602 (2012).
 M. Eschrig and T. Lofwander, Triplet Supercurrents in Clean and Disordered Half-Metallic Ferromagnets, Nat. Phys.4, 138 (2008).
 E. C. Gingrich, P. Quarterman, Yixing Wang, R. Loloee, W. P. Pratt, Jr., and N. O. Birge,Spin-Triplet Supercurrent in Co=NiMultilayer Josephson Junctions with Perpendicular Anisotropy,Phys. Rev. B86, 224506 (2012).
 J. W. A. Robinson, J. D. S. Witt, and M. G. Blamire, Con-trolled Injection of Spin-Triplet Supercurrents into a Strong Ferromagnet,Science329, 59 (2010).
 S. Mironov and A. Buzdin, Triplet Proximity Effect in Superconducting Heterostructures with a Half-Metallic Layer,Phys. Rev. B92, 184506 (2015).
 R. S. Keizer, S. T. B. Goennenwein, T. M. Klapwijk, G. X. Miao, G. Xiao, and A. Gupta,A Spin Triplet Supercurrent through the Half-Metallic Ferromagnet CrO2, Nature (London)439, 825 (2006).
 M. S. Anwar, F. Czeschka, M. Hesselberth, M. Porcu, and J. Aarts, Long-Range Supercurrents through Half-Metallic FerromagneticCrO2,Phys. Rev. B82, 100501 (2010).  A. Singh, S. Voltan, K. Lahabi, and J. Aarts, Colossal
Proximity Effect in a Superconducting Triplet Spin Valve Based on the Half-Metallic FerromagnetCrO2,Phys. Rev. X5, 021019 (2015).
 X. L. Wang, A. Di Bernardo, N. Banerjee, A. Wells, F. S. Bergeret, M. G. Blamire, and J. W. A. Robinson, Giant Triplet Proximity Effect in Superconducting Pseudo Spin Valves with Engineered Anisotropy, Phys. Rev. B 89, 140508(R) (2014).
 P. G. Ivanov, S. M. Watts, and D. M. Lind,Epitaxial Growth ofCrO2Thin Films by Chemical-Vapor Deposition from a Cr8O21 Precursor,J. Appl. Phys.89, 1035 (2001).  H. A. Bullen and S. J. Garrett, Epitaxial Growth ofCrO2
Thin Films onTiO2 (110) Surfaces,Chem. Mater.14, 243 (2002).
 See Supplemental Material at http://link.aps.org/ supplemental/10.1103/PhysRevX.6.041012 for details of pendeoepitaxy growth and the correlation between vertical and lateral overgrowth.
 X. Zou and G. Xiao,Magnetic Domain Configurations of Epitaxial Chromium Dioxide (CrO2) Nanostructures,Appl. Phys. Lett.91, 113512 (2007).
 A. Tanaka, R. Chen, K. L. Jungjohann, and S. A. Dayeh, Strong Geometrical Effects in Submillimeter Selective Area Growth and Light Extraction of GaN Light Emitting Diodes on Sapphire,Sci. Rep.5, 17314 (2015).
 A. Gupta, X. W. Li, S. Guha, and G. Xiao,Selective-Area and Lateral Overgrowth of Chromium Dioxide (CrO2) Films by Chemical Vapor Deposition, Appl. Phys. Lett.
75, 2996 (1999).
 C. König, M. Fonin, M. Laufenberg, A. Biehler, W. Bührer, M. Kläui, U. Rüdiger, and G. Güntherodt,Micromagnetism and Magnetotransport Properties of Micron-Sized Epitaxial CrO2 (100) Wires,Phys. Rev. B75, 144428 (2007).  A. Biehler, M. Kläui, M. Fonin, C. König, G. Güntherodt,
and U. Rüdiger, Micromagnetism and Magnetotransport Properties of Micron-Sized Epitaxial CrO2 (100) Wires, Phys. Rev. B75, 184427 (2007).
 W. M. Martinez, W. P. Pratt, and N. O. Birge, Amplitude Control of the Spin-Triplet Supercurrent in S=F=S Josephson Junctions,Phys. Rev. Lett.116, 077001 (2016).  M. S. Anwar and J. Aarts,Anomalous Transport in Half-Metallic Ferromagnetic CrO2, Phys. Rev. B 88, 085123 (2013).
 P. Dubos, H. Courtois, B. Pannetier, F. K. Wilhelm, A. D. Zaikin, and G. Schön,Josephson Critical Current in a Long Mesoscopic S-N-S Junction,Phys. Rev. B63, 064502 (2001).  S. P. Lewis, P. B. Allen, and T. Sazaki,Band Structure and Transport Properties ofCrO2,Phys. Rev. B55, 10253 (1997).  T. Koyama, D. Chiba, K. Ueda, K. Kondou, H. Tanigawa, S. Fukami, T. Suzuki, N. Ohshima, N. Ishiwata, Y. Nakatani, K. Kobayashi, and T. Ono, Observation of the Intrinsic Pinning of a Magnetic Domain Wall in a Ferromagnetic Nanowire,Nat. Mater.10, 194 (2011).